Compressive Response of Concrete
Confined with Steel Spirals
and FRP Composites
J.-Y. LEE,1 C.-K. YI,2,* H.-S. JEONG,3 S.-W. KIM4 AND J.-K. KIM1
1Department of Architectural Engineering, Sungkyunkwan University
300, Chunchun-dong, Jangan-gu, Suwon 440-746, Republic of Korea
2School of Civil, Environmental, and Architectural Engineering
Korea University, Anam-dong, Seongbuk-gu, Seoul 136-713, Republic of Korea
3Construction Engineering Service Network Co., 833-2 Yeoksam-dong
Kangnam-gu, Seoul 135-933, Republic of Korea
4Department of Architectural Engineering, Kongju National University
275 Budae-dong, Cheonan 330-717, Republic of Korea
ABSTRACT: This article presents the results of an experimental and analytical
study on the behavior of concrete cylinders externally wrapped with fiber-reinforced
polymer (FRP) composites and internally reinforced with steel spirals. The experi-
mental work was carried out by testing twenty-four 150� 300mm2 concrete cylin-
ders subjected to pure compression with various confinement ratios and types of
confining material. The test results show that the compressive response of concrete
confined with both FRP and steel spirals cannot be predicted by summing the
individual confinement effects obtained from FRP and steel spirals. This is largely
attributable to differences in the inherent material properties of FRP and steel.
A new empirical model to predict the axial stress�strain behavior of concrete
confined with FRP and steel spirals is proposed. Comparisons between experimental
results and theoretic predictions show agreement.
KEY WORDS: fiber-reinforced polymer, lateral confining pressure, confined
concrete, steel spiral, deformability, concrete cylinder.
IN THE LAST two decades, the use of fiber-reinforced polymer (FRP) composites hasdrawn much attention in the civil engineering community, which faces stringent new
design requirements and demands for lower cost . FRP has proven itself as the material
of choice to meet these new needs with its many favorable properties, such as a high
strength-to-weight ratio, effective corrosion resistance, and ease of on-site handling and
*Author to whom correspondence should be addressed. E-mail: [email protected]
Journal of COMPOSITE MATERIALS, Vol. 44, No. 4/2010 481
0021-9983/10/04 0481�24 $10.00/0 DOI: 10.1177/0021998309347568
� The Author(s), 2010. Reprints and permissions:
application in confined spaces resulting in reduced labor costs. It has been demonstrated
that lateral confinement increases compression strength, deformability, and energy
absorption capacity of concrete [2,3]. Effective lateral confinement can be achieved by
wrapping FRP composite around the perimeter of a concrete member.
Early attempts to use FRP composites as confining materials in columns were performed
by Kurt  and Fardis and Khalili [5,6]. These attempts were followed by many experimen-
tal studies to investigate the effects of FRP spirals [7,8], FRP wraps [9�19], and FRP tubes
[20�23] on the compressive response of concrete columns. The early analytical model used
to predict the compressive response of concrete confined with FRP composites closely
follows the models derived for steel confinements (spirals, hoops, or ties) . However,
such models yield inaccurate and often unconservative results . Improved mathematical
models have been proposed to capture FRP and concrete material behaviors and to predict
the compressive response of concrete confined with FRP composites [26�28].
Most of the previous experimental and analytical studies focus on the compressive
response of concrete confined with either FRP composites or steel spirals. In reality,
when reinforced concrete (RC) columns are wrapped with FRP composites, the core
concrete is confined simultaneously by two different confining materials as follows: the
FRP composites and the steel reinforcements already present in the column, as shown in
Figure 1(a) . If both confining materials are similar in their stress�strain behaviors,
then the compressive response of concrete confined with the two materials (e.g., steel
spirals and FRP composites) can be predicted using the models developed for a single
confining material with the equivalent confinement ratio of the external and internal
reinforcements. However, the stress�strain behavior of steel is quite different from that
of FRP composites.
Strain of concrete
by steel spiral
Strain of concrete
Strain of concrete
by steel spiral
Figure 1. Compressive response of concrete confined by various materials: (a) concrete column, (b)
stress�strain curve of concrete confined by steel spiral, (c) stress�strain curve of concrete confined by
FRP, and (d) stress�strain curve of concrete confined by both steel spiral and FRP.
482 J.-Y. LEE ET AL.
The stress�strain curve of steel exhibits an initial linear-elastic stage followed by a
yielding plateau, in which the tensile strain increases with little increase in stress.
In contrast, the tensile stress�strain curve of FRP composites remains linear elastic
until the final brittle rupture. Figure 1(b) and (c) depict the compressive stress�strain
curves of steel spiral-confined concrete and FRP-confined concrete, respectively, and
clearly demonstrate the differences between their behaviors. The compressive stress�strain
curve of concrete confined with steel spirals shows loss of stiffness before it reaches its
maximum strength, after which the compressive response follows a gradual post-peak
descending branch, and the failure strength is typically lower than the peak strength.
On the other hand, the compressive stress�strain curve of FRP-confined concrete presents
a nearly bilinear response, as shown in Figure 1(c). Therefore, when concrete is confined
by these two materials, a link between the confinement effects of the different materials
must be established.
The confinement effect of different material was also investigated by Liu et al.  who
tested concrete columns to investigate the confinement effect of fiber-reinforced compo-
sites fabricated by filament winding method with various combinations of hybrid fibers
and lay up angles on the compressive strengths of concrete. According to Liu et al.’s test
results, the compressive strengths of concrete columns were influenced by the combination
of hybrid fibers. For example, concrete columns confined by the foil-glass�Kevlar-glass
(FGKG) hybrid composites were stronger than those reinforced by the foil-glass�carbon-
glass (FGCG) hybrid composites. However, Liu et al.’s hybrid fibers were resin cured and
essentially became a single confining composite material around the concrete cylinder
before the compressive test; hence, the analysis of the effect of each fiber type on the
concrete compressive behavior was limited.
This article presents the results of an experimental and analytical study on the perfor-
mance of concrete cylinders externally wrapped with FRP sheets and internally reinforced
with steel spirals. Twenty-four 150� 300mm2 concrete cylinders are tested under pure
compression. Applied load, axial strain, and lateral strain are recorded to monitor the
stress�strain behavior, ultimate strength, and corresponding strain of the tested specimens.
The experimental results are then compared with some of the existing confinement models
available in the technical literature. In addition, a new analytical model to predict the
behavior of concrete confined with both FRP and steel is proposed.
A total of twenty-four 150� 300mm2 cylindrical specimens were prepared from the
same concrete mix. The cylinders were divided into four series with four different steel
confinement ratios (�ls ¼ 4Asp=ðds � sÞ, where Asp is the cross-sectional area of the steel
spiral, s is the pitch of spirals, and ds is the distance between the centers of the spiral, 130
mm), as given in Table 1 in which the test specimens are designated with two letters, S and
F for the steel confinement and the FRP confinement, respectively. The numeric digits
following the letters S and F designate the pitch of the steel spiral ties in centimeters and
the number of layers of the FRP composite applied, respectively. For example, specimen
S0F0 indicates that this cylinder was neither confined with steel spiral hoops nor FRP
sheets, while S2F4 indicates that this cylinder was confined with both the steel spiral ties
Compressive Response of Concrete 483
having a pitch of 2 cm and four layers of the FRP composite. The pitch of spirals was
varied from 20�60 mm. The steel spirals were made of 5.0 �mm diameter bars and had the
yield strength of 1200MPa. The cross-sectional area of the spiral (Asp) is 19.63 mm
series consists of six cylinders, each with a different FRP confinement ratio (�lf ¼ 4t=D,
where t is the thickness of the FRP composites and D is the diameter of cylinder). FRP
sheets had a thickness of 0.11 mm and a tensile strength of 4500 MPa. The layer of FRP
sheets was varied from 0 to 5 (Table 1).
The concrete cylinders were removed from the forms af